Share this document with a friend

24

Transcript

1

Simulation of Avalanche Photodiodes Using APSYSSimulation of Avalanche

Photodiodes Using APSYS

Copyright 2006-7 Crosslight Software Inc.www.crosslight.com

2

ContentsContentsContents

APSYS model for APD simulationModeling of InP/InGaAs SAGCM APDModeling of InGaAs/AlGaAs RCE SAGCM APDHot carrier model of GaAs/ AlGaAs PIN APDSummary

APSYS model for APD simulationModeling of InP/InGaAs SAGCM APDModeling of InGaAs/AlGaAs RCE SAGCM APDHot carrier model of GaAs/ AlGaAs PIN APDSummary

3

APSYS model for APD simulationDrift-diffusion and hydrodynamic models:

Drift-diffusion model (DD): Poisson’s equation and electron/hole continuity equations.

Hydrodynamic model (HD): Poisson’s equation, electron/hole continuity equations and carrier energy balance equations.

Optically induced carrier generation rate computed from absorption spectra based on interband transition model or imported externally.

Transfer matrix method with improved theoretical expressions to deal with light beams propagating through multiple layers.

Both small signal AC and large signal models available. The latter is preferred because effect of carrier screening is more significant at large signal.

Various numerical techniques were developed to help convergence near breakdown.

4

APSYS model for APD simulation

])/(exp[)(, mcEA εεβα −=

Impact ionization & excess noise factorImpact ionization models: Baraff’s phonon scattering theory or Chynoweth’s

empirical formulas. Carrier energy dependence is used for HD model.

Excess noise factor usually calculated usually calculated vsvs APD multiplication gain M according APD multiplication gain M according to McIntyreto McIntyre’’s expression:s expression:

where where kkeffeff= = αα//ββ is the ratio of electron/hole impact ionization coefficients. is the ratio of electron/hole impact ionization coefficients. The coefficients may be computed directly by the APSYS program oThe coefficients may be computed directly by the APSYS program or r obtained from field distribution using the obtained from field distribution using the ChynowethChynoweth model:model:

Resonant conditionπψψλπ mLn bft 24 =++

Here ψf and ψb are the phase shifts due to the penetration of lightwaves into the top and bottom mirror regions, respectively. Lt is the total cavity length.

5

ContentsContentsContents

APSYS model for APD simulationModeling of InP/InGaAs SAGCM APDModeling of InGaAs/AlGaAs RCE SAGCM APDHot carrier model of GaAs/ AlGaAs PIN APDSummary

6

InP/InGaAs SAGCM APD structure

Central region were declared Central region were declared ““activeactive”” so that absorption so that absorption coefficient were computed by APSYS. Grading layer coefficient were computed by APSYS. Grading layer

between between InGaAs InGaAs & & InPInP were used. were used.

7

Band diagram & optic power distributionBand diagram at equilibrium (zero Band diagram at equilibrium (zero bias), 2bias), 2ndnd column along ycolumn along y--direction.direction.

Plot shows absorption in Plot shows absorption in InGaAsInGaAsregion. Soregion. So--called separate called separate

absorption, grading, charge & absorption, grading, charge & multiplication (SAGCM) multiplication (SAGCM)

structure.structure.

8

2D relative optic power density & optic generation rate

2D relative energy within the 2D relative energy within the device. Absorption mostly in device. Absorption mostly in InGaAsInGaAs region.region.

PhotoabsorptionPhotoabsorption generated generated electronelectron--hole pair happens in hole pair happens in

InGaAsInGaAs absorption region.absorption region.

9

Electric field profile & impact ionizationHigh electric field in the High electric field in the InPInP multimulti--plicationplication region & low electric field region & low electric field in the absorption region.in the absorption region.

Impact ionization rate (at 30V) mostly Impact ionization rate (at 30V) mostly in the in the InPInP multiplication region.multiplication region.

10

Excess noise factor & I-V curves

Photocurrent and dark current. Photocurrent and dark current. Breakdown voltage near 30.45 V.Breakdown voltage near 30.45 V.

Excess noise factor computed based on Excess noise factor computed based on McIntyreMcIntyre’’s expression and impact s expression and impact ionization coefficients.ionization coefficients.

11

Multiplication gainScale photocurrent by Scale photocurrent by the photocurrent where the photocurrent where impact ionization just impact ionization just starts to get starts to get multiplimultipli--cationcation gain, or gain, or alternaalterna--tivelytively take the ratio of take the ratio of area under the impulse area under the impulse response curve with response curve with impact ionization over impact ionization over the one without impact the one without impact ionization. The gain ionization. The gain values obtained by the values obtained by the two methods agree two methods agree usually with each other usually with each other as long as enough time as long as enough time length for impulse length for impulse response is taken.response is taken.

Multiplication gain Multiplication gain vsvs reverse bias extracted from the photo IV curve.reverse bias extracted from the photo IV curve.In good agreement with experiment In good agreement with experiment ((Bandyopadhyay Bandyopadhyay et al, IEEE J. et al, IEEE J.

Quantum Electron. 34 (4), pp. 691Quantum Electron. 34 (4), pp. 691--699 (1998)699 (1998)).).

12

Impulse response

Impulse response is fast Fourier transformed (FFT) to frequency Impulse response is fast Fourier transformed (FFT) to frequency responseresponsefrom which the from which the ––3 dB bandwidth is evaluated.3 dB bandwidth is evaluated.

13

Bandwidth

Consistent with experiment Consistent with experiment ((BandyopadhyayBandyopadhyay et al, IEEE J. Quantum et al, IEEE J. Quantum EletronEletron..34 (4), pp. 69134 (4), pp. 691--699 (1998)699 (1998)).).

14

ContentsContentsContents

15

RCE SAGCM APD structure

Schematic Schematic InGaAsInGaAs//AlGaAsAlGaAs RCE SAGCM APD structure and RCE SAGCM APD structure and schematic layer view generated byschematic layer view generated by CrosslightCrosslight APSYS simulator APSYS simulator (see (see H H NieNie et al, et al, IEEE Photon. IEEE Photon. TechnolTechnol. . LettLett.. 10, pp. 40910, pp. 409--411, 1998; Y G 411, 1998; Y G XiaoXiao et al, et al, J. J. Lightwave TechnolLightwave Technol.. 19, pp. 101019, pp. 1010--1022, 2001 )1022, 2001 )..

16

Band diagram & relative optic energy density

Band diagram Band diagram (equilibrium, zero bias)(equilibrium, zero bias)

Resonant standing waves are clearly observed at Resonant standing waves are clearly observed at the absorption region within the cavity.the absorption region within the cavity.

17

Optic generation rate & quantum efficiency

Enhanced absorption at the absorption layer & two neighbor Enhanced absorption at the absorption layer & two neighbor grading layers is observed.grading layers is observed.

Peak QE Peak QE 68.4%, QE asymmetry due to the neighbor 2nd order 68.4%, QE asymmetry due to the neighbor 2nd order (left) resonance peak for the (left) resonance peak for the GaAsGaAs--AlAsAlAs mirror structures usedmirror structures used(see K (see K KishinoKishino et al et al IEEE J Quantum Electron.IEEE J Quantum Electron. 27, pp. 202527, pp. 2025––2034, 1991).2034, 1991).

18

I-V curves & multiplication gain

Unity gain at ~5.6V, & breakdown at ~ 17.6 V.Unity gain at ~5.6V, & breakdown at ~ 17.6 V.

Modeled multiplication gain consistent with the experimental Modeled multiplication gain consistent with the experimental (see (see H H NieNie et al, et al, IEEE Photon. IEEE Photon. TechnolTechnol. . LettLett.. 10, pp. 40910, pp. 409--411, 1998)411, 1998)..

19

Impulse response & bandwidth

GainGain--bandwidth product limit: taking long time to achieve the bandwidth product limit: taking long time to achieve the peak response & long relaxation time back to the dark backgroundpeak response & long relaxation time back to the dark backgroundat large reverse biases.at large reverse biases.

Bandwidth generally consistent with the experimental (need Bandwidth generally consistent with the experimental (need detailed Cdetailed C--V profile for more accurate modeling at low gain region)V profile for more accurate modeling at low gain region)(Experimental see K (Experimental see K KishinoKishino et al et al IEEE J Quantum Electron.IEEE J Quantum Electron. 27, pp. 202527, pp. 2025––2034, 1991)2034, 1991)..

20

ContentsContentsContents

21

GaAs/AlGaAs PIN APD structure

Intrinsic AlIntrinsic Al.6.6GaGa.4.4As As layer for energylayer for energybuildup purposebuildup purpose

See: Kwon et al, J. See: Kwon et al, J. LightwaveLightwaveTechnolTechnol. . VolVol 23 No 523 No 5(2005) pp 1896(2005) pp 1896--19061906

p++ 30-nm GaAs(~1e19 cm-3)

p+ 800-nm GaAs(5e18 cm-3)

i “x”-nm Al(.6)Ga(.4)As

i 200-nm GaAs

n+ 300-nm GaAs(5e18 cm-3)

n+ GaAs Substrate

22

Band diagram & impact ionization rate

Hot electron effect shrinks the effective multiplication Hot electron effect shrinks the effective multiplication region since there is no ionization in the dark space (or region since there is no ionization in the dark space (or

low energy region).low energy region).

Band diagram at equilibrium (zero Band diagram at equilibrium (zero bias).bias).

23

I-V curves & bandwidthHigh bias needed to achieve the same High bias needed to achieve the same multiplication gain with hot electron multiplication gain with hot electron effect.effect.

The simulator predicted more realistic The simulator predicted more realistic bandwidth with hot electron effect.bandwidth with hot electron effect.

24

SummaryModeling of Modeling of InPInP//InGaAs InGaAs SAGCM APD, SAGCM APD, InGaAs/AlGaAs RCE SAGCM APD and and GaAsGaAs//AlGaAs AlGaAs PIN APD presented with PIN APD presented with comparison with experiment or other theory.comparison with experiment or other theory.

Typical physical properties like band diagram, photoTypical physical properties like band diagram, photo--absorption & generation, impact ionization & electric field absorption & generation, impact ionization & electric field profile, & performance characteristics like photoprofile, & performance characteristics like photo-- & dark& dark--current, multiplication gain, excess noise factor, impulse current, multiplication gain, excess noise factor, impulse response, & response, & --3 dB bandwidth etc., presented for most of the 3 dB bandwidth etc., presented for most of the simulatedsimulated APDsAPDs..

Computed multiplication gain and bandwidth are consistent Computed multiplication gain and bandwidth are consistent with the experimental for with the experimental for InPInP//InGaAsInGaAs SAGCM SAGCM APD and APD and InGaAs/AlGaAs RCE SAGCM APD..

Some techniques for modeling also introduced. The APSYS Some techniques for modeling also introduced. The APSYS could predict more realistic bandwidth with hot electron could predict more realistic bandwidth with hot electron effect.effect.

Recommended